Flexural Behaviour of Mono Fibre and Hybrid
Fibre Reinforced Concrete using Steel and Nylon
Jyothis Jose Oommen Mr. Tom George
P.G. Student Assistant Professor
Department of Civil Engineeing Department of Civil Engineeing
Mar Baselios College of Engineering and Technology Mar Baselios College of Engineering and Technology
This paper presents an experimental study on the effect of hybrid fibre addition to M40 concrete mix using the steel-nylon hybrid fibre reinforced system. The study is done by comparing the flexural behaviour of reinforced concrete beams without fibres, with steel fibres, with nylon fibres and with hybrid fibre combination of steel and nylon. M40 grade concrete was designed as the control mix. The main variables considered were the volume fraction of crimped steel fibres and nylon fibres. The mechanical properties of the mono fibre reinforced cast specimens were tested at four different volume fractions of fibre content i.e., 0.5%, 1.0%, 1.5% and 2.0%. The optimum volume fraction of steel fibre addition was obtained as 1.5% and that of nylon fibre addition was obtained as 1%. Hybrid combinations of 1.5% by volume of steel fibre along with various volume fractions of nylon fibre, such as 0.1%. 0.15%, 0.2%, 0.25% and 0.3%, were cast in order to find the optimum percentage of the hybrid steel-nylon fibre combination. An optimum of hybrid combination of 1.5% steel with 0.2% of nylon was obtained. A total of 12 reinforced concrete beams were cast and tested. After conducting flexural strength test on the beams, the first crack load, deflection pattern, crack development pattern and ultimate load carrying capacity of the beams were studied and compared.
Keywords: Civil Engineering, Concrete, Fibres, Flexure, Hybrid, Steel-Nylon, Structural Engineering
Concrete is a tension-weak building material, which is often crack ridden connected to plastic and hardened states, drying shrinkage, and so on. The cracks generally develop with time and stress to penetrate the concrete, thereby impairing the waterproofing properties and exposing the interior of the concrete to the destructive substances containing moisture, bromine, acid sulphate, etc. The exposure acts to deteriorate the concrete, with the reinforcing steel corrosion. To counteract the cracks, a fighting strategy has come into use, which mixes the concrete with the addition of discrete fibres. Plain cement concrete has some shortcomings like low tensile, limited ductility, little resistance to cracking, high brittleness poor toughness, and so on that restrict its application. The cracking of concrete may be due to economic structural, environmental factors, but most of the cracks are formed due to inherent internal micro cracks and the inherent weakness of the material to resist tensile forces. Drying shrinkage in the concrete may also results in the formation of cracks. To overcome these deficiencies, extra materials are added to improve the performance of concrete.
Fibre reinforced concrete provides solutions for these shortcomings. Inclusion of fibres as reinforcement to concrete results as crack arrestor and improves its static and dynamic properties by preventing the propagation of cracks as well as increases tensile strength of concrete. Extensive research work on FRC during the last two decades has established that combination of two or more types of fibres such as metallic and non-metallic fibres increase overall performances of concrete. It is obvious that the behaviour of HFRC depends on the aspect ratios, orientations, geometrical shapes, distributions and mechanical properties of fibres in concrete mixtures. Fibre-reinforced concrete are mostly used for on-ground floors and pavements, but can be considered for a wide range of construction parts (beams, piers, foundations etc.) either alone or with hand-tied rebars. Investigations to overcome the brittle response and limiting post – yield energy absorption of concrete led to the development of fibre reinforced concrete (FRC) using discrete fibres within the concrete mass. The fibres were introduced to develop concrete with enhanced flexural and tensile strength. The fibres were included in the concrete is to delay and control the tensile cracking of the composite materials. The fibres, thus transform inherent unstable tensile crack propagation into a slow controlled crack growth. The fibre reinforcement delays the initiation of flexural and shear crack. It strongly influences the post cracking behaviour and significantly enhances the toughness of the composite.
compression, tension, flexure, etc. High strength concrete with single fibres of either type does not offer a significant improvement in mechanical properties. Hence in recent years, there has been research on hybrid fibre reinforced concrete which incorporates the advantages of both types of fibres in a single matrix.
In order to achieve the main research goal, a systematic approach was set out by fulfilling some main objectives. The specific objectives of the study are enumerated below.
1) To find the optimum volume fractions of steel, nylon and hybrid combination of steel and nylon fibres.
2) To assess the mechanical properties of mono fibre reinforced and hybrid fibre reinforced concrete, target compressive strength at the age of 28 days being around 48 MPa.
3) To analyse the flexural properties of mono fibre reinforced and hybrid fibre reinforced concrete beam.
Materials Used: A.
The materials used in this study were: 1) Portland Puzzolona cement 2) Manufactured sand
3) Coarse aggregate with a maximum size of 20mm
4) Superplasticizer – a High Range Water Reducing Agent (HRWRA) 5) Crimped steel fibre of aspect ratio 66 (length-30mm; diameter-0.45mm) 6) Monofilament nylon fibre of aspect ratio 160 (length-40mm; diameter-0.25mm) Test results of Cement:
Portland Pozzolana Cement, confirming to IS 1489 (Part 1) – 1991 (Reaffirmed 2005), was used throughout this investigation. The different laboratory tests were conducted on cement as per IS 12269: 1987
Table – 1 Properties of Cement
Properties Test Results
Standard consistency 34%
Compressive strength 33 MPa
Initial setting time 1hr 5mins
Final setting time 5hrs 20mins
Specific gravity 3.15
Test Results of Fine Aggregate: C.
Commercially available Manufactured Sand passing through 4.75 mm IS sieve which conforms to IS specification was used as fine aggregate. Laboratory tests were conducted to determine the different physical properties as per IS 383 – 1970 specifications. The test results conforms the M- sand to zone II of IS 383 – 1970 recommendations.
Table – 2
Properties of Fine Aggregate
Properties Result obtained
Fineness modulus 2.96
Specific gravity 2.5
Fig. 1: Gradation Curve of Fine Aggregate
Test Results of Coarse Aggregate: D.
Crushed aggregate with a maximum size of 20 mm was used for preparing the mixes. On performing sieve analysis, it was observed that the coarse aggregate confirms to IS specification, i.e. it lies within the required zone. The test results confirm to IS 383-1970 (part III) recommendations.
Table – 3
Properties of Coarse Aggregate
Properties Result obtained
Fineness modulus 7
Bulk density 1.6
Void ratio 0.27
Specific gravity 2.9
A High Range Water Reducing Agent, Cera hyperplast XR-W40, which is a polycarboxylate ether based superplasticizer was used for the work and its specification compliance is as per ASTM C 494-03, BS 5075 and IS 9103.
Details of the Designed Mix: F.
Table – 4
Mix Proportion of the Conventional Mix
Materials By Weight By Proportion
Cement 394 kg/m3 1
Fine Aggregate 657.288 kg/m3 1.668
Coarse Aggregate 1324.314 kg/m3 3.3612
Water 157.6 kg/m3 0.4
Superplasticer 1.527 kg/m3 0.00387
Slump obtained: 145mm
7th day Compressive Strength: 31.2 MPa 28th day Compressive Strength: 48.88 MPa
Table – 5
Specimen Identification Details
Specimen Id Specimen Details
CM Control mix (without fibres)
SFRC Steel Fibre Reinforced Concrete
NFRC Nylon Fibre Reinforced Concrete
HFRC Hybrid Steel- Nylon Fibre Reinforced Concrete
The effect of steel fibres was studied by adding 0.5%, 1%, 1.5% and 2% by volume of 0.45 mm diameter steel fibres with aspect ratio 66 to the designed mix. The variations in fresh and hardened properties due to the addition of steel fibre on the mix are tabulated in Table 4. The workability decreased and the hardened properties such as cube compressive strength, cylinder compressive strength and modulus of elasticity increased with addition of fibres. Since the primary objective of fibre addition was improvement in tensile and flexural behaviour, optimum performance was observed for concrete with 1.5% of steel fibre addition. Hence for further study the percentage of steel fibre addition was fixed as 1.5%.
Table – 6
Fresh and Hardened Properties of SFRC Mix
Designation of Specimen
Compressive Strength (N/mm2)
Split Tensile Strength (N/mm2)
Flexural Strength (N/mm2)
CM 0 145 48.8 3.02 3.6
SFRC1 0.5 120 50.7 3.13 4.2
SFRC2 1 114 46.8 3.25 5.4
SFRC3 1.5 110 43.7 3.53 6
in the case of SFRC. The values are tabulated in Table 5. Optimum performance was observed for the mix with 1% of nylon fibre addition.
Table - 7
Fresh and Hardened Properties of NFRC Mix
Designation of Specimen Fibre Percentage (%) Slump (mm) Compressive Strength (N/mm2)
Split Tensile Strength (N/mm2)
Flexural Strength (N/mm2)
CM 0 145 48.8 3.02 3.6
NFRC1 0.5 130 49.6 1.92 4.8
NFRC2 1 124 51.6 2.83 5.2
NFRC3 1.5 119 52.2 2.68 4.6
NFRC4 2 112 48.8 2.26 4.0
The influence of hybrid fibres on the mix was studied by adding nylon fibres at 0.1%, 0.15%, 0.2%, 0.25% and 0.3% by volume with the optimum content of steel fibre which is 1.5% by volume. From the test results tabulated in Table 6, it was found that even though workability decreased with the addition of nylon fibres, there was excellent improvement in hardened properties such as flexural strength and tensile strength. The optimum percentage of hybrid combination of steel and nylon was found to be 1.5% of steel with 0.2% of nylon by volume.
Table - 8
Fresh and Hardened Properties of HFRC Mix
Designation of Specimen Optimum Steel fibre percentage (%) Nylon fibre content (%) Slump (mm) Compressive Strength (N/mm2)
Split Tensile Strength (N/mm2)
Flexural Strength (N/mm2)
CM 0 0 145 48.8 3.02 3.6
SFRC3 1.5 0 110 43.7 3.53 6
HFRC1 1.5 0.1 106 48.2 3.6 7
HFRC2 1.5 0.15 103 52.1 3.8 7.4
HFRC3 1.5 0.2 100 50.8 4.3 8
HFRC4 1.5 0.25 95 49.8 3.1 6.4
HFRC5 1.5 0.3 91 47.7 3 5.6
12 RC beam specimens of length 1 m and cross section 100 mm x 150 mm were prepared. Two specimens, each, were prepared for control mix (CM), mix with optimum steel fibre content (SFRC), mix containing optimum nylon fibre content (NFRC) and mix containing optimum content of hybrid steel-nylon fibre (HFRC). The beams were designed as under reinforced sections. The reinforcement details consists of 2-10 mm dia. Bars at the tension face, and 2-8mm dia. Bars at the compression face. The fibres were reinforced in the plastic region of concrete (Figure 3). The plastic hinge length was determined using the formula given below.
Lp = 0.08 L + 0.022 db fy Where, L = length of the member (mm)
db = diameter of the rebar (mm)
Fig. 3: Fibre Reinforced Concrete In Plastic Region Of The Beam
All the beams were cured for 28 days. The behaviour of the beams was studied under two point loading, on a 1000 kN universal testing machine. The schematic diagram of test setup is shown in Figure 4.
Fig. 4: Test Setup for Beams
A dial gauge was used to determine the mid span deflection. Two LVDTs were used to measure the strain. The beams were tested under two point loading. The values obtained from the dial gauge at the mid span were used to plot the load deflection curve. LVDTs were used to measure the strains. These strain values were used for plotting the moment curvature relationship.
TEST RESULTS AND DISCUSSIONS
The results of the flexural tests on RC Beams are discussed in this section. The load-deflection characteristics, energy absorption capacity, moment curvature relationship, first crack load, ductility index, crack pattern, and ultimate load were obtained.
Load Deflection Behaviour: A.
Fig. 5: Load Deflection Graph
The figure shows the load – deflection behaviour of RC beams without fibres (CM) and with optimum fibre content of steel (SFRC), nylon (NFRC) and hybrid combination of steel and nylon (HFRC). The dial gauges were placed at the bottom of the tested beams, and hence, the values were obtained only after the beams underwent elastic deformation in the downward direction. The load deflection curve shows that for all the specimens, the curve was linear up to the first crack load. Further application of load makes the curve deviate from linearity. This is due to the formation of multiple cracks. Further with a slight increase in load, the steel was found to yield and the curve becomes flat till the ultimate load was reached. The load deflection plots of CM and NFRC were almost the same while that of HFRC and SFRC were better in response. The deflections of the beams were observed with the formation of initial crack after which the deflection remained almost linear up to a certain load level. Then the deflection became nonlinear, and the slope of the graph decreased. The peak deflection at the ultimate load was obtained, and the value further increased in the unloading phase. Due to experimental limitations, the deflection in the unloading phase was only obtained till 80% of the ultimate load.
Energy Absorption Capacity: B.
Energy absorption is found by the area under the load deflection plot. The energy absorption of different specimens are shown in Table 7.
Table – 9
Energy Absorption of Beams Mix Energy Absorption (kN mm)
Moment Curvature Relationship: C.
Fig. 6: Moment Curvature Relationship
Figure 6 shows the moment curvature plot for the beams. The moment curvature can be said to have three stages. First stage is till cracking, second stage till yielding of tension steel and the third stage to limit of useful strain in concrete. The curve is linear up to first crack moment. Further when the moment increases, the curve shifts from linearity. When the moment reaches yield moment, the curves become flat. When steel yields, a large increase in curvature occurs with a small change in moment.
First Crack Load, Yield Load and Ultimate Load: D.
The yield moment and the yield load was calculated using necessary equations. The yield load for all the beams were found to be in the same range. The ultimate load was found experimentally. The results are tabulated in Table 8.
Table – 10
Ultimate Yield and First Crack Load
Mix Initial Crack Load (kN) Yield Load (kN)
Ultimate Load (kN)
CM 17.5 45.48 67.5 1
NFRC 12.5 43.3 70 1.03
SFRC 22.5 46.2 72.5 1.07
HFRC 25 46.5 78 1.15
It can be seen that, FRCs are having a higher ultimate value compared to the CM. 16 % increase in ultimate load was observed in HFRC when compared to that of CM. SFRC and NFRC are having ultimate load of about 7.5 % and 4% higher than that of CM.
Ductility Index: E.
Displacement ductility was calculated as the ratio of the displacement at ultimate load to the displacement at yield load. Failure of an under reinforced beam is called tension failure. This is because the primary reason of failure is the yielding of steel bars. The large increase in curvature, before collapse of the beam is an indication of ductile failure of beam. Curvature ductility was calculated as the ratio of curvature at ultimate load to that of curvature at yield load. The ductility index of the beams are shown in Table 9.
Displacement Ductility Curvature Ductility
Absolute Relative Absolute Relative
CM 2.24 1 2.59 1
NFRC 2.3 1.03 3.09 1.19
SFRC 2.76 1.23 4.86 1.87
HFRC 4.27 1.91 31.08 12
Addition of fibres improved the ductility of beams. High value of ductility shows the ability to undergo large inelastic deformation without any reduction in strength.
Crack Pattern: F.
Fig. 7: Crack Pattern of CM Beams Fig. 8: Crack Pattern of NFRC Beams
Fig. 9: Crack Pattern of SFRC Beams Fig. 10: Crack Pattern of HFRC Beams
Following conclusions are drawn from the experimental investigations conducted to assess the influence of fibres on the flexural response of the beams.
1) Fresh concrete properties of the designed mix, such as workability and flowability decreased while the hardened properties such as compressive strength, flexural strength and tensile strength improved by the addition of fibres. 2) The optimum percentage of steel fibre addition was 1.5% by volume and that of nylon fibre was 1% by volume. The
optimum content of the hybrid combination was 1.5% of steel with 0.2% of nylon fibre by volume.
3) The first crack load increased with addition of fibres. The first crack load of steel fibre reinforced beam increased by 29% and that of hybrid fibre reinforced beams increased by 43% when compared to that of control mix beams. While that of NFRC decreased by 28% when compared to that of control mix beams.
4) Deflection was reduced by the presence of fibres by 6%, 5% and 4% in the case HFRC, SFRC and NFRC, respectively, when compared to CM.
6) The energy absorption capacity of SFRC, NFRC and HFRC was increased by 7.5%, 4% and 21%, respectively, when compared to that of CM
7) The energy absorption capacity is more for hybrid fibre reinforced beams and hence it is more ductile. 8) All the beams exhibited similar trend of crack propagation and failed by yielding of tensile reinforcement and
subsequent crushing of concrete in the compression zone.
9) From the analysis it was obvious that the first crack load, pre-cracking and post-cracking behaviour, deflection pattern, crack development pattern and ultimate load carrying capacity of the concrete beams improved with fibre addition and this improvement is more pronounced in hybrid fibre reinforced (HFRC) beams.
10) The fibre reinforced beams, in general, exhibited better ductile behaviour than beams without fibres.
 Ganesan, N., Raj, J. and Shashikala, A., P., "Strength and Behaviour of Steel Fibre Reinforced Self Compacting Concrete in Flexure," Proceedings of the International Conference on Advanced in Concrete composites and Structures, 2013.
 Yung, W., Yung, L. and Hua, L., Bending and Uniaxial Tensile Test on Concrete Reinforced with Hybrid Steel Fibres”, Journal of Materials in Civil Engineering, September 2013, pp 519-527.
 Akcay, B. and Tasdemir, M., “Definition and measurement of flexural toughness parameters for fibre reinforced concrete” 2012.
 El-Dieb, A, S., and Reda, T, M., “Super plasticizers and entraining Agents State of the art and future needs”, Concerte Technology Past present and future, Proceedings of V. Mohar Malhotra symposium, Vol. 144, 2012, pp 399-416.
 Gao, X., Feng, Y., L., and Yan, Y., “Introduction to Steel Fibre Reinforced Concrete on Engineering Performance of Concrete” International Journal of Scientific & Technology Research Vol. 1, No. 4, May 2012.
 Mazin Burhan Adeen and Alya’a Abbas Al-Attar., “Determination of Mechanical Properties of Hybrid Steel-Nylon Fiber Reinforced Concrete”, Modern Applied Science, Vol. 4, No. 12, 2010, pp 97–109.
 Zhean, L. U., FAN Xiaochun and CHEN Yingbo., “Mechanical Properties of Layered Steel Fiber and Hybrid Fiber Reinforced Concrete”, Journal of Wuhan University of Technology, Vol. 23, No. 5, 2008, pp. 733-737.
 Xiang, Gao B. Eng., “Mix design and impact response of fibre reinforced and plain reactive powder concrete”, M.Sc. Thesis, RMIT University, 2007.  Sulaiman, M. and Collepardi M., “Recycling of industrial waste performance of steel concrete”, J cent south university, Vol. 16, 2006, pp 768-773.  Du¨zgu¨n, O. A., Gul, R., Aydin, A. C., “Effect of steel fibres on the mechanical properties of natural lightweight aggregate concrete”, Materials Letters.
Vol. 59, 2005, pp 3357 – 3363.
 Najim, K. and Hall, M., “Materials and properties of Fibre Reinforced Concrete” Proceedings of the international symposium on FRC, 2005.
 Banthia, N. and Nandakumar, N., “Crack Growth Resistance of Hybrid Fibre-Reinforced Cement Composites,” Cementitious Concrete Composite, Vol. 25, No. 1, 2003, pp. 3-9.